arXiv:1701.03656v1 [cond-mat.mes-hall] 13 Jan 2017

Instituto Federal de Educa¸c˜ao, Ciˆencia e Tecnologia Baiano - Campus Senhor do Bonfim, Km 04 Estrada da Igara, 48970-000 Senhor do Bonfim, Bahia, Brazil

Abstract Magnetic nanowires have been considered to compose devices based on the concepts of spintronic and magnonic technologies. Despite stripe and cylindrical nanomagnets being widely studied, curvature effects on the magnetic properties of nanowires have been low explored. In this work the analysis of the influence of curvature on the demagnetizing field inside a curved magnetic wire is proposed. By performing analytical calculations, it is shown that unlike their cylindrical counterparts, curved nanowires present a demagnetizing field that has different values along its polar-like angle. In addition, the demagnetizing field presents a dependence on the azimuthal position.

1

I.

INTRODUCTION

Due to their potential applications in random access memory, data storage1 , cancer therapy2 , spintronic and magnonic devices3 , magnetic nanoparticles have been widely studied, as from experimental as from theoretical point of view. From experimental point of view, several works have reported the production and characterization of nanomagnets with different shapes and sizes4–6 . For instance, recent advances in experimental techniques to fabricate nanoparticles has made it possible the production of nanomagnets with unusual geometries such as rolled-up magnetic membranes7 , paraboloidal magnetic caps8 or modulated nanomagnets9 . The production of nanomagnets with cylindrical geometry (nanowires and nanotubes) has been also reported10 . Such magnetic nanowires and nanotubes appear as prominent candidates to compose units of information for non-volatile memories, logic gates11,12 and devices based on the concept of “race-track memory”13 . This development on experimental techniques to produce magnetic nanoparticles and the possibilities of applications for such structures make it necessary the understanding on the influence of curvature on the magnetic properties of nanoparticles. In this context, in last years, a lot of effort has been done aiming to describe how the geometry can influence the properties of nanomagnets20,21 . The proposition of a race-track device demands the understanding on the dynamics of a domain wall along a nanowire. In the case of cylindrical nanowires, the knowledge on the dynamics of domain wall under the action of magnetic fields or spin currents is reasonably well developed14–17 . Among main results, interesting properties appearing due to the symmetry of cylindrical nanowires are theoretically predicted and experimentally observed. Among them, the absence of a Walker field18 in the domain wall motion can be highlighted. Indeed, unlike what it is noted for stripe nanowires19 , the domain wall moves smoothly in a cylindrical nanowire and its velocity does not present the oscillatory behavior occurring above the Walker field15 . On the other hand, due to the lost of cylindrical symmetry, interesting magnetic properties are noted if the cylindrical nanowire is curved. For example, it was shown that a domain wall can be pinned even when it is passing across curved region of a nanowire22 . In addition, torsion and curvature effects lead to the appearance of a Walker limit and negative velocities during the domain wall motion23,24 . Based on the above and on the influence of the geometry on the magnetic properties of nanomagnets, in this work 2

it is proposed the study of the dependence of the demagnetizing field on the geometry of a curved nanowire. It is well known that the demagnetizing field of an in-plane single domain state in a cylindrical nanowire is independent on the direction in which the magnetization is pointing in25 . On the other hand, once the cylindrical symmetry is lost in a curved wire, the demagnetizing field of a homogeneous magnetization configuration must present a dependence on the curvature. Indeed, by representing a curved wire as a torus section, the demagnetizing fields of four different magnetization configurations are obtained and it is shown that the components of the demagnetizing field present an explicit dependence on the curvature. This work is divided as follows: in Section II we present the adopted theoretical model to describe the nanowire and to calculate the demagnetizing field; Section III brings the results and discussions; finally, in Section IV the conclusions and prospects are presented.

II.

THEORETICAL MODEL

The main objective of this work is to determine the demagnetizing field generated inside a curved wire described as a torus section. In this case, the micromagnetic theory will be adopted. In the frame of micromagnetism, a magnetic structure is described as a continuous medium whose magnetic state is defined by the magnetization vector as a function of the position inside the element. In this case, the demagnetizing field can be calculated by H = −∇Φ, where Φ is the magnetostatic potential, determined from the Laplace equation ∇2 Φ = 0. In the absence of electric currents, the magnetostatic potential comes from surface and volumetric magnetic charges, respectively defined as σ = m · n and % = ∇ · m. Here, ~ /MS , with n is the normal vector pointing outward the surface of the magnet and m = M M being the magnetization vector and MS the saturation magnetization. In this case, the formal solution of the Laplace equation is given by MS Φ= 4π

Z S

σ dS − |~r − ~r 0 |

Z V

% dV |~r − ~r 0 |

,

(1)

where |~r 0 − ~r| is the distance between two points into the magnetic body. Since a curved magnet is being considered, all vector operators must be given in a curvilinear basis26 . Then, in order to calculate the magnetostatic potential of a curved wire, it 3

FIG. 1. Adopted coordinate system to describe the curved wire.

will be paramettrized by a torus section, that is27 ~r = xˆ

ρ sinh β cos ϕ ρ sinh β sin ϕ ρ sin η + yˆ + zˆ , cosh β − cos η cosh β − cos η cosh β − cos η

(2)

where ρ is a constant that defines the radius of a circle in the plane z = 0 when β → ∞. β ∈ [β0 , ∞) determines the torus thickness (β0 describes the external surface), ϕ ∈ [−ϕ0 , ϕ0 ] plays the role of an azimuthal angle and η ∈ [0, 2π] is the poloidal angle (See Fig. 1). The coordinate system represented in Eq. (2) can be related to a more natural parameters describing a torus by cosh β = R/r (the external surface of the wire is described by cosh β0 = √ R/r) and ρ = R2 − r2 , where r and R are the poloidal and toroidal radii28 , respectively. The wire length is given by ` = 2ϕ0 R in such way that the wire with greater curvature, described by a half-torus section, is obtained when (ϕ0 = π/2 → R = `/π) and an almost straight wire is obtained for R → ∞. From Eq. (2), one can evaluate the normal vector ˆ − G(β, η)ˆ pointing outward the wire surface, obtaining n = −βˆ = −F (β, η)R z , where F (β, η) ≡ F =

1 − cosh β cos η cosh β − cos η

(3)

and G(β, η) ≡ G = −

sinh β sin η . cosh β − cos η

(4)

ˆ = xˆ cos ϕ + yˆ sin ϕ is the radial vector pointing outward the wire in the In addition, R xy-plane. 4

FIG. 2. Considered magnetization configurations. (a) describes a SDx state; (b) a SDz state; (c) represents a RSD state; and (d), a VSD state.

~ ≡ MS m is parametrized in a spherical coordinate system (r, φ, θ) The magnetization M on the basis of Cartesian coordinates, that is, m = xˆ cos φ sin θ+ yˆ sin φ sin θ+ zˆ cos θ. For the purposes of this work, the demagnetizing fiels associated with four different magnetization configurations (see Fig. 2) will be calculated: i) a single domain state pointing along x direction (SDx), described by mSDx = xˆ; ii) a single domain state pointing along z-zxis direction (SDz), where mSDz = zˆ; iii) a radial single domain state (RSD), in which the ˆ and an inmagnetic moments pointing outward the wire and are described by mRSD = R; surface state (HV), in which the magnetic moments point along azimuthal direction of the wire, mHV = ϕˆ = −ˆ x sin ϕ + yˆ cos ϕ. These magnetic states have been chosen because they share general features of other magnetic configurations that can appear as magnetization groundstate or metastable states in a curved nanowire. The calculation of the magnetostatic potential is, in general, very hard. A possible way is expanding the inverse of the distance in an infinite series using Green’s functions. In the case of toroidal geometry, the inverse of the distance in toroidal coordinates is given by27 p ∞ (cosh β 0 − cos η 0 )(cosh β − cos η) X 1 = (−1)k εn εk cos n(η 0 − η) |~r 0 − ~r| πρ k,n=0 × cos k(ϕ0 − ϕ)

Γ(n − k + 1/2) k P (cosh β< )Qkn−1/2 (cosh β> ) , Γ(n + k + 1/2) n−1/2

(5)

k where εk = (2 − δk,0 ), εn = (2 − δn,0 ), Γ(x) is the gamma function, Pn−1/2 (cosh β) and

Qkn−1/2 (cosh β) are the Legendre functions of half-integer order (also known as toroidal harmonics). From using the expansion given in Eq. (5), the magnetostatic potential for single domain29 and onion30 states in magnetic nanotori were obtained. In some situations, it is useful to describe the components of a vector field in their Cartesian components. In this context, the components of a vector field (H) writen in 5

toroidal coordinates (β, η, ϕ) can be changed to a Cartesian basis (x, y, z) by using the transformation

Hx

Hy Hz

F cos ϕ G cos ϕ − sin ϕ

= F sin ϕ G sin ϕ cos ϕ G −F 0

Hβ

Hη , Hϕ

(6)

where F and G were defined in Eq. (3).

III.

RESULTS

From the presented model, analytical expressions for the magnetostatic potential and the demagnetizing fields associated to each magnetization configuration can be determined.

A.

Magnetostatic potential

There are two contributions to the magnetotatic potential associated to SDx state. The first contribution comes from the ends of the wire, that is, at −ϕ0 (S1 ) and ϕ0 (S2 ), where mSDx · ϕˆ = − sin ϕ0 . The second contribution comes from magnetostatic charges appearing along the wire external surface (β0 ) and given by mSDx · n = −F cos ϕ. Thus, the magnetostatic potential of SDx is given by ΦSDx = ΦSDx1 + ΦSDx2 , where Z Z MS sin ϕ0 sin ϕ0 ΦSDx1 = − dS1 + dS2 , 4π r 0 − ~r| r 0 − ~r| S2 |~ S1 |~

(7)

and ΦSDx2

MS = 4π

Z S3

1 cos ϕ(cosh β0 cos η − 1) dS3 , |~r 0 − ~r| (cosh β0 − cos η)

(8)

where the integrals are evaluated at the wire surface. The surface element along the wire external surface is dS3 = ρ2 sinh β0 /(cosh β0 − cos η)2 dηdϕ, while the surface element at the wire ends is dS1 = dS2 = ρ2 /(cosh β − cos η)2 dηdβ. The integral in ϕ must be evaluated in the interval ϕ ∈ [−ϕ0 , ϕ0 ]. In this case, the substitution of Eq. (5) in Eqs. (7) and (8) yields √ ∞ ΦSDx1 ρ cosh β 0 − cos η 0 X k =− (−1)k εn εk gk (ϕ0 ) Pn−1/2 (cosh β 0 ) MS 2π 2 k,n=0 Z ∞ Z 2π cos n(η − η 0 ) −k × dβ Qn−1/2 (cosh β) dη , (cosh β − cos η)3/2 β0 0 6

(9)

and √ ∞ cosh β 0 − cos η 0 X k (−1)k εn εk fk (ϕ0 )Pn−1/2 (cosh β0 ) 2 4π k,n=0 Z 2π cos n(η − η 0 )(cosh β0 cos η − 1) −k ×Qn−1/2 (cosh β) dη , (cosh β0 − cos η)5/2 0

ρ sinh β0 ΦSDx2 = MS

(10)

where gk (ϕ0 ) = sin ϕ0 cos kϕ0 cos kϕ0 , fk (ϕ0 ) =

2 cos kϕ0 (k sin kϕ0 cos ϕ0 − cos kϕ0 sin ϕ0 ) . k2 − 1

(11)

and we have used the property31 Γ(n − k + 1/2) k 0 Q (cosh β 0 ) = Q−k n−1/2 (cosh β ) , Γ(n + k + 1/2) n−1/2

(12)

The integrals in η can be performed from using the trigonometric identity cos n(η 0 − η) = cos nη cos nη 0 + sin nη sin nη 0 and the integral representation of Qkn−1/2 (cosh β) (See Ref.27 p. 961). In this case, after some algebraic manipulation, we have that ΦSDx1 =

∞ X p k cos nη 0 Ωk,n (β0 )gk (ϕ0 ) Pn−1/2 (cosh β 0 ) , cosh β 0 − cos η 0

(13)

k,n=0

and ΦSDx2

∞ X p 0 0 0 = cosh β − cos η cos nη 0 Λk,n (β0 )fk (ϕ0 )Q−k n−1/2 (cosh β ) ,

(14)

k,n=0

where 2ρ MS Ωk,n (β0 ) = π2

√

2

k

Z

∞

(−1) εn εk

dβ β0

1 Q−k n−1/2 (cosh β) Qn−1/2 (cosh β)

sinh β

,

(15)

and √

2 cosh β0 k 0 (−1)k εn εk Pn−1/2 2 3π " 20 # 2 0 Qn+1/2 Q n−1/2 0 × − n Q1n−1/2 − , sinh β0 sinh β0

Λk,n (β0 ) = −

with P (Q)νµ

0

2ρ MS

(16)

≡ P (Q)µν (cosh β0 ).

The calculation of the magnetostatic potential of the SDz configuration follows the same procedure above described. However, in this case, the ends of the wire do not contribute to the magnetostatic potential. Thus, the magnetostatic potential of this configuration is Z MS ρ2 sinh β sinh β sin η ΦSDz = dηdϕ . (17) 4π S3 |~r 0 − ~r| (cosh β − cos η)3 7

Then, analogously to the performed calculations to determine ΦSDx2 , we have that ΦSDz =

∞ X p 0 cosh β 0 − cos η 0 n sin nη 0 Ψk,n (β0 ) hk (ϕ0 ) Q−k n−1/2 (cosh β ) ,

(18)

k,n=0

where Ψk,n (β0 ) = −

8ρ MS

√ 2 sinh β0 0 k 0 (−1)k εn εk Q1n−1/2 Pn−1/2 3π 2

(19)

and hk (ϕ0 ) = k −1 (2 cos kϕ0 sin kϕ0 ). The third configuration consists in a radial state. As the SDz state, RSD has no surface magnetostatic charges at the ends of the wire. However, there are two contributions to the magnetostatic potential. One coming from surface and other coming from volumetric charges. That is, ΦRSD = ΦRSDS + ΦRSDV , where subscripts S and V denote surface and volumetric contributions to the magnetostatic potential. From the definition of the magnetization in RSD state, it can be noted that mRSD · n = −F . Then, the calculation of the surface contribution to the magnetostatic potential is promptly obtained from the expression of ΦSDx2 with the replacement of fk (ϕ0 ) by hk (ϕ0 ). Then, ΦRSDS

∞ X p 0 0 0 cos nη 0 Λk,n (β0 )hk (ϕ0 )Q−k = cosh β − cos η n−1/2 (cosh β ) .

(20)

k,n=0

The volumetric charge associated to RSD state is determined from the divergent of the magnetization written in curvilnear coordinate system26 , ∇ · mRSD = (cosh β − cos η)/ρ sinh β. is obtained

Therefore, after some algebraic manipulation, the following expression √ ∞ X ρ MS 2 p 0 0 ΦRSDV = cosh β − cos η (−1)k εn εk cos nη 0 π2 k,n=0 Z ∞ Q1 −k n−1/2 (cosh β) Qn−1/2 (cosh β) 0 k 0 ×hk (ϕ ) Pn−1/2 (cosh β ) dβ sinh β β0 ∞ X 1p 0 0 cosh β − cos η cos nη 0 Ωk,n (β0 ) ⇒ ΦRSDV = 2 k,n=0 k × hk (ϕ0 ) Pn−1/2 (cosh β 0 ) .

(21)

At last, it will be analyzed the magnetostatic potential of a VSD configuration. In this case, only the surface charges associated to the ends of the wire accounts to the calculations and thus, the magnetostatic potential of VSD state is given by ΦV SD = − 8

ΦSDx1 . sin ϕ0

(22)

B.

Demagnetizing fields

Despite having analyzed the magnetostatic potential of four different magnetization configurations, due to their similar expressions, in this subsection only the demagnetizing field of RSD and SDz states will be evaluated. The results here obtained give a good qualitative description for the two other states. By using the ∇ operator in toroidal coordinates27 , the demagnetizing field in a toroidal coordinate system is evaluated as 1 ∂Φ 0 cosh β 0 − cos η 0 ∂Φ ˆ0 ∂Φ 0 β + 0 ηˆ + ϕˆ . Hd = − ρ ∂β 0 ∂η sinh β 0 ∂ϕ0

(23)

Therefore, the demagnetizing field in a toroidal basis can be represented as Hd = Hβ βˆ + Hη ηˆ + Hϕ ϕ. ˆ In this case, the components of the demagnetizing field associated to surface charges of RSD state are given by √

HβSRSD ×

n sinh β 2

Q−k n−1/2 (cosh β) + (cosh β − cos η) √

HηS RSD

∞ cosh β − cos η X =− cos nη Λk,n (β0 )hk (ϕ) ρ k,n=0

=−

o dQ−k n−1/2 (cosh β)

,

dβ

(24)

∞

cosh β − cos η X Λk,n (β0 )hk (ϕ)Q−k n−1/2 (cosh β) ρ k,n=0 n1 o × sin η cos nη − n(cosh β − cos η) sin nη , 2

(25)

and HϕSRSD

∞ (cosh β − cos η)3/2 X dhk (ϕ) =− cos nη Λk,n (β0 )Q−k . n−1/2 (cosh β) ρ sinh β dϕ k,n=0

(26)

The components of the demagnetizing field associated to the volumetric charges of RSD configuration are √

HβVRSD ×

n sinh β 2

HηVRSD

∞ cosh β − cos η X =− cos nη Ωk,n (β0 )hk (ϕ) 2ρ k,n=0

k Pn−1/2 (cosh β)

+ (cosh β − cos η)

k dPn−1/2 (cosh β) o

dβ

,

√ ∞ cosh β − cos η X k =− Ωk,n (β0 )hk (ϕ)Pn−1/2 (cosh β) 2ρ k,n=0 n1 o × sin η cos nη − n(cosh β − cos η) sin nη , 2 9

(27)

(28)

and HϕVRSD

∞ dhk (ϕ) (cosh β − cos η)3/2 X k . cos nη Ωk,n (β0 )Pn−1/2 (cosh β) =− 2ρ sinh β dϕ k,n=0

(29)

Since the magnetostatic potential of SDx configuration (Eqs. (10) and (14)) has similar expressions to the magnetostatic potential of RSD state (Eqs. (20) and (21)), qualitative behavior of the demagnetizing field for SDx state is well described by the previously presented results. Then, explicit equations of the demagnetizing field associated with SDx configuration will be omitted here. The solution of the magnetostatic potential of SDz state (See Eq. (18)) presents subtle differences when compared with Eq. (20). In this context, it is interesting to perform the explicit calculation of the demagnetizing field related to this configuration, which is evaluated as √ HβSDz = − ×

n sinh β 2

∞ cosh β − cos η X n sin nη Ψk,n (β0 )hk (ϕ) ρ k,n=0

Q−k n−1/2 (cosh β)

+ (cosh β − cos η)

o dQ−k n−1/2 (cosh β) dβ

,

(30)

√

HηSDz

∞ cosh β − cos η X n Ψk,n (β0 )hk (ϕ)Q−k =− n−1/2 (cosh β) ρ k,n=0 n1 o × sin η sin nη + n(cosh β − cos η) cos nη , 2

(31)

and HϕSDz

C.

∞ dhk (ϕ) (cosh β − cos η)3/2 X =− n sin nη Ψk,n (β0 )Q−k . n−1/2 (cosh β) ρ sinh β dϕ k,n=0

(32)

Numerical results

Despite having obtained analytical expressions for the demagnetizing field components given in Eqs. (24)-(32), an immediate analysis of their physical content is not clear due to their complicated forms. Therefore, to extract relevant results we should evaluate them numerically. For doing that, we employ the Fortran subroutine code DTORH132,33 , which k gives the values of Pn−1/2 (cosh β) and Qkn−1/2 (cosh β). Due to the fast convergence of the

series, we stop the sums at k = 30 and n = 30. 10

In this work, the results are normalized in relation to the saturation magnetization, that is, in numerical calculations MS = 1 is adopted. In addition, the poloidal radius and length of the nanowires are respectively r = 10 nm and ` = 100 nm. The toroidal radius R is varied in function of ϕ0 , in the form R = `/2ϕ0 . Consequently, the wire with greater curvature, K = 1/R = π × 107 m−1 , is given by a half-torus section (ϕ0 = π/2). The presented numerical results describe the demagnetizing field on the wire surface (β = β0 ). Figs. 3-(a) and (b) present respectively the dependence of HβRSD on the curvature and on the azimuthal position, ϕ, along the wire. From Fig.3a, it can be noted that HβRSD depends on the curvature of the wire. In this case, the graphics show a cosine-like behavior and an asymmetry for η = 0 and η = π is observed. That is, the absolute value of HβRSD at η = 0 is lower than its absolute value at η = pi. Then, ∆HβRSD = HβRSDη=0 − HβRSDη=π < 0. Nevertheless, it is interesting to note that the smaller the curvature, the smaller ∆HβRSD , in such way that ∆HβRSD → 0 when 1/K → 0. On the other hand, despite small quantitative variations, qualitative changes of HβRSD are no observed at different positions along the wire (See Fig. 3-(b)). Figs. 3-(c) and (d) present the behavior of HηRSD for different curvatures and different positions along the wire. It can be noted a sine-like behavior with maxima absolute values given at η = π/2 and η = 3π/2. Despite HηRSD is depending on curvature, no asymmetry is observed when we compare its maximum absolute values at η = π/2 and η = 3π/2. Finally, the behavior of HϕRSD in function of the position along the wire is shown in Fig. 3-(f). It can be noted that HϕRSD = 0 in the center of the wire (ϕ = 0) and increases, in absolute value, reaching its maximum value at the wire ends. The maximum value of the demagnetizing field appearing in the internal border of the wire shows an interesting relation between curvature and dipolar energy. This effect must be important in describing the properties of a domain wall displacing along curved wires. However, curvature effects on the dypolar field is a low explored issue. In general, most of works devoted to study this theme use the space of momenta to calculate the demagnetizing field of curved particles34–37 . In Fig. 4 it is presented the components of the demagnetizing fields of SDz configuration, obtained from Eqs. (30) - (32). Analogously to what happens for RSD state, the demagnetizing field depends on the curvature of the wire. However, there is a reversal in the behavior of Hβ and Hη . That is, HβSDz presents a sine-like behavior and its absolute value is symmetric under the change from η = π/2 to η = 3π/2. On the other hand, HηSDz presents a cosine-like behavior with a maximum value (in absolute value) at η = π. 11

FIG. 3. Components of the demagnetizing field of RSD state for different curvatures and azimuthal positions along the curved wire in function of η. (a) and (c) show, respectively, HβRSD and HηRSD at ϕ = 0 for different curvatures. (b) and (d) show the dependence of HβRSD and HηRSD on the azimuthal position ϕ along the wire for a constant curvature. Fig. (e) shows the behavior of the function f (η) = HηRSD cos η − HβRSD sin η. (f) shows the dependence of HϕRSD on the azimuthal position along the wire for a constant curvature.

12

FIG. 4. Components of the demagnetizing field of SDz state for different curvatures in function of η. (a) shows the behavior of HβSDz and (b) presents HηSDz at ϕ = 0 for different curvatures.

FIG. 5. Fig. (a) presents the component along x-axis direction in function of η for different curvatures. Fig. (b) shows the demagnetizing field pointing along z-zxis direction for the SDz state.

The representation of the demagnetizing fields in a Cartesian basis can lead to a more intuitive description of the demagnetizing field of a curved wire. By using Eq. (6), we can numerically calculate the components HxRSD and HzSDz . The analysis of Fig. 5 evidences the dependence on the curvature of the demagnetizing fields, as well as the maximum (absolute value) of the demagnetizing fields at η = π. It can be noted that HxRSD decreases with the decreasing of curvature and its value tends to a constant for 1/K → 0. This behavior is noted also for HzSDz . This curvature-dependent demagnetizing field can produce differences in the magnetization groundstate of nanowires when they are curved. Furthermore, a domain wall displacing 13

along a curved nanowire must present curvature-induced changes in its dynamics. In fact, Yershov et al 22 showed that a domain wall can be pinned by a curved region in a cylindrical nanowire. However, in that work, the observed effects are purely related with exchange energy cost. Here, we show that dipolar field can also produce observable effects on the magnetic properties of a curved wire.

IV.

CONCLUSIONS

Analytical solutions to the magnetostatic potential of four magnetization configurations (SDx, SDz, RSD and VSD) have been obtained by representing a curved wire as a torus section. For considering a curvilinear basis, the demagnetizing field of two of the considered configurations (RSD and SDz) have been explicitly calculated. The obtained results evidence a dependence of the demagnetizing field on the curvature of the wire. Furthermore, despite its angular symmetry along poloidal direction, the absolute values of the demagnetizing fields are different at the external and internal borders of the wire. The dependence on the curvature of the demagnetizing field is also evidenced when the demagnetizing field components are written in terms of a Cartesian basis. The obtained solutions are important to describe the magnetization groundstate configuration and the properties of a domain wall in a curved wire. The author thanks the financial support of the Brazilian agencies CNPq (301015/2015-5) and Fapesb (JCB0063/2016). He thanks also D. Altbir and A. Espejo for fruitful discussions and suggestions.

∗

vagson.carvalho@usachcl

1

R. Hertel, Nat. Nanotechnol. 8, 318 (2013).

2

D.-H. Kim, E. Rozhkova, I. Ulasov, S. Bader, T. Rajh, M. Lesniak, and V. Novosad, Nature Mater. 9, 165 (2009).

3

A.P. Guimar˜ aes, Principles of Nanomagnetism, (Springer, Heidelberg, 2009).

4

R. P. Cowburn, D. K. Koltsov, A. O. Adeyeye, M. E. Welland, D. M. Triker, Phys. Rev. Lett. 83 , 1042 (1999).

14

5

F. Q. Zhu, G.W. Chern, O. Thernyshyov, X.C. Zhu, J.G. Zhu, and C.L. Chien, Phys. Rev. Lett. 96 , 027205 (2006).

6

R. P. Cowburn, J. Phys. D 33, R1 (2000).

7

R. Streubel, D.J. Thurmer, D. Makarov, F. Kronast, T. Kosub, V.P. Kravchuk, D.D. Sheka, Y. Gaididei, R. Schfer, and O.G. Schmidt, Nano Lett. 12, 3961 (2012).

8

D.W. Shi, P.K. Greene, P. Liu, K. Javed, K. Liu, and X. F. Han, IEEE Trans. on Magnetics 50, 2303004 (2014).

9

I. Minguez-Bacho, S. Rodriguez-L´ opez, M. V´azquez, M. Hern´andez-V´elez, and K. Nielsch, Nanotechnology 25, 145301 (2014).

10

M. V´azquez, in Advanced Magnetic Nanowires ed. by H. Krom¨ uller, and S. Parkin, Handbook of Magnetixm and Advanced Magnetic Materials, vol. 4 (Wiley, Chichester, 2007).

11

J. jaworowicz, N. Vernier, J. Ferr´e, A. Maziewski, D. Stanescu, D. Ravelosona, A.S. Jacqueline, C.Chappert, B. Rodmac, and B. Di´eny, Nanotechnology 20, 215401 (2009).

12

D.A. Allowood, G. Xiong, C.C. Faulkner, D. Atkinson, D. Petit, and R.P. Cowburn, Science 309, 1688 (2005)

13

S.S.P. Parkin, M. Hayashi, and L. Thomas, Science 320, 190 (2008);

14

Y.P. Ivanov, M. V´ azquez, and O.Chubykalo-Fesenko, J. Phys. D. 46, 485001 (2013).

15

M. Yan, A. K´ akay, S. Gliga, and R. hertel, Phys. Rev. Lett. 104, 057201 (2010).

16

R. Wieser, E.Y. Vedmedenko, P. Weinberger, and R. Wiesendanger, Phys. Rev. B 82, 144430 (2010).

17

R. Hertel, and A. K´ akay, J. Magn. Mag. Mat. 379, 45 (2015).

18

N.L. Schryer, and L.R. Walker, J. Appl. Phys. 45, 5406 (1974).

19

A. Mougin, M. Cormier, J.P. Adam, P.J. Metaxas, and J. Ferr´e, Europhys. Lett. 78, 57007 (2007).

20

Y. Gaididei, V.P. Kravchuk, and D.D. Sheka, Phys. Rev. Lett. 112, 257203 (2014).

21

R. Streubel, P. Fischer, F. Kronast, V.P. Kravchuk, D.D. Sheka, Y. Gaididei, O.G. Schmidt, and D. Makarov, J. Phys. D 49, 363001 (2016).

22

K.V. Yershov, V.P. Kravchuk, D.D. Sheka, and Y. Gaididei, Phys. Rev. B 92, 104412 (2015).

23

K.V. Yershov, V.P. Kravchuk, D.D. Sheka, and Y. Gaididei, Phys. Rev. B 93, 094418 (2016).

24

O.V. Pylypovskyi, D.D. sheka, V.P. Kravchuk, K.V. Yershov, D. Makarov, and Y. Gaididei, Sci. Rep. 6, 23316 (2016).

15

25

A. Aharoni, IEEE Trans. on Magnetics 27, 3539 (1991); L. Kraus, Czech. J. Phys. B 23, 512 (1973).

26

G.B. Arfken, and H.J. Weber, Mathematical Methods for Physicists, 6th ed. (Elsevier Academic Press, 2005).

27

P. Morse, and H. Feshbach, Methods of Theoretical Physics, (M Graw-Hill, New York, 1953).

28

S. Vojkovic, A.S. Nunez, D. Altbir, and V.L. Carvalho-Santos, J. Appl. Phys. 120, 033901 (2016).

29

M. Bellegia, M. De Graef, and Y.T. Millev, Proc. R. Soc. A 465, 3581 (2009).

30

V.L. Carvalho-Santos, W.A. Moura-Melo, and A.R. Pereira, J. Appl. Phys. 108, 094310 (2010).

31

I.S. Gradshteyn, and I.M. Ryzhik, Table of Integral, Series and Products, 7th ed. (Academic, New York, 2007).

32

J. Segura, and A. Gil, Comput. Phys. Commun. 124, 104 (2000).

33

J. Segura, and A. Gil, Comput. Phys. Commun. 139, 186 (2001).

34

M. Bellegia, J.W. Lau, M.A. Shofield, Y. Zhu, S. Tandon, M. De Grael, J. Magn. Mag. Mat. 301 , 131 (2006).

35

M. Beleggia, M. De Graef, J. Magn. Mag. Mat. 263, L1 (2003).

36

S. Tandon, M. Beleggia, Y. Zhu, M. De Graef, J. Magn. Mag. Mat. 271, 27 (2004).

37

M. Beleggia, M. De Graef, J. Magn. Mag. Mat. 285, L1 (2004).

16